the reduction-coupled oxo activation mechanistic motif .the reduction-coupled oxo activation...
Post on 12-Jun-2018
Embed Size (px)
The Reduction-Coupled OxoActivation mechanistic motif forCH bond activation and oxidation
Reproduced in part with permission from:
1. Cheng, M.-J.; Fu, R.; Goddard, W. A. III. Chem. Commun. 2014, 50, 17481750. c 2014
The Royal Society of Chemistry; available at http://dx.doi.org/10.1039/C3CC47502F;
2. Cheng, M.-J.; Goddard, W. A. III.; Fu, R.; Nielsen, R. J. Top. Catal., in press. Unpublished
work c 2014 Springer.
Also includes original work.
The vanadium phosphorus oxide (VPO) catalyst is used commercially for the selective oxidation of
n-butane to maleic anhydride. Surprisingly, the mechanism has been shown to initiate with CH
activation by a PO moiety. In this chapter, we call this phenomenon the Reduction-Coupled Oxo
Activation (ROA) mechanistic motif, and attribute it to the concomitant formation of a strong
oxo-hydrogen bond on the phosphorus atom and a one-electron reduction on the vanadium atom.
In addition, we show that the same ROA phenomenon can be extended beyond phosphorus and
vanadium to additional main-group elements and transition metals, respectively, and may lead to a
new strategy in designing selective catalysts for alkane activation. Finally, we propose the existence of
a homogeneous vanadium phosphorus oxo complex that can incorporate the novel ROA mechanistic
pathway as a potential propane oxidation catalyst. We considered several oxidation pathways leading
to end products such as propylene, isopropanol, and propylene oxide. We support our assertions with
density functional theory calculations on potential reaction pathways.
4.2.1 The VPO catalyst for n-butane oxidation
Vanadium phosphorus oxide (VPO) is an inorganic complex that catalyzes the oxidation of n-
butane to maleic anhydride with a surprisingly high selectivity of 60-70%  (Scheme 4.1). Although
the overall yield is only ca. 50%, its ease of synthesis, use of common elements, and selectivity
have allowed this catalyst to be commercialized, producing ca. 500 kilotons of maleic anhydride
annually . Hence, there was a strong impetus to investigate the mechanism of this reaction in the
hopes of rationally designing a modified catalyst with improved yield.
Scheme 4.1. The oxidation of n-butane to maleic anhydride using vanadium phosphorus oxide as a catalyst.
A useful parameter for the CH activating ability of each oxo moiety in the catalyst is the
H-atom affinity DH, which is defined as the enthalpy change when the OH bond in MOH is
homolytically cleaved to form the MO oxo. Mechanistic work initially centered on vanadyl py-
O)2(P2O7), abbreviated VOPO), the major component of VPO . However, it
was quickly found that no vanadium oxo on the VOPO surface has sufficient H-atom affinity to
activate n-butane (Figure 4.1). The most active VO in VOPO has a DH value of 58.2 kcal/mol,
whereas the weakest CH bond in n-butane has a dissociation energy of 89.3 kcal/mol, implying
an extremely endothermic first step that is categorically inconsistent with the experimentally deter-
mined activation energy of 12.9-23.6 kcal/mol . Hence, it was concluded that the reduced vanadyl
O)2(P2O7) alone is unable to initiate the catalytic process.
Figure 4.1. OH bond strength for oxygen atoms on the (VIVO)2(P2O7) surface. The energy released whenan H is bound to the VO (in red) is only 58.2 kcal/mol, not nearly high enough for alkane activation tooccur. The energy released when an H is bound to the bridging VOP oxide (in green) is even lower, at17.0 kcal/mol. The energy released when an H is bound to the PO was not determined because geometryoptimization caused it to be transferred to the VOP moiety (in green).
It was then supposed that catalysis requires the presence of adsorbed O2 on the VIVO(P2O7)
surface. Adsorption of O2 may be molecular, in which the OO bond is retained, two VIV centers
are oxidized to VV, and a vanadium peroxo moiety is formed; or it may be dissociative, in which
the OO bond is broken and four VIV centers are oxidized to VV. The first case is uphill by 2.8
kcal/mol, whereas the second is downhill by 38.8 kcal/mol. Unfortunately, the DH values calculated
for the resulting vanadium peroxo and vanadium oxo moieties were only 70.0 and 58.9 kcal/mol,
respectively. Hence, it was concluded that the reduced VPO complex is not the active catalyst.
Figure 4.2. Oxygen adsorption energies on the (VIVO)2(P2O7) surface and the OH bond strength (DH)to each of these O atoms. Left: molecular O2 adsorption in which the OO bond is preserved. Right:dissociative adsorption in which the OO bond is broken. All energies are in kcal/mol.
Finally, it was proposed that catalysis takes place on a metastable VVOPO4 surface, known
as the X1 phase, which has been experimentally determined to be produced in the high oxygen
environment of the reaction conditions . However, the largest DH value found for a vanadium
oxo in this phase is only 62.8 kcal/mol (Figure 4.3). Surprisingly though, it was discovered that
the phosphorus oxo had a much larger DH value of 84.3 kcal/mol! This implies a first step that is
endothermic by only 5.0 kcal/mol, with an activation energy later calculated to be 13.6 kcal/mol,
which is within the experimental range. The stability of the resulting monohydrogenated species was
attributed to the fact that spin density appears to be localized on the neighboring vanadium atoms
4.2.2 The ROA mechanistic motif
The surprising discovery of the CH activation ability of PVO moieties in the VVOPO4 catalyst led
to the creation a new term, Reduction-Coupled Oxo Activation (ROA), to describe this phenomenon.
Its usefulness is due to the observation that the basicity of simple transition metal oxos increases
with decreasing electron affinity of the metal, due to increasing electron density; whereas for CH
activation it is preferred that both basicity and electron affinity are maximized, since H-atom transfer
Figure 4.3. OH bond strengths for the various oxygen atoms on the X1-VVOPO4 surface. The OH bondstrength of 84.3 kcal/mol to the PO moiety leads to a first step that is endothermic by only 5.0 kcal/mol,with an activation energy later calculated to be 13.6 kcal/mol. Hence, the PO moiety is the only candidatesite whose CH activation energy is compatible with experimental data.
Figure 4.4. CH activation by a phosphorus oxo leads to a one electron reduction on the neighboring vana-dium. Hence the oxidation state of the phosphorus atom does not change. (a) Vanadium-phosphate archetype:conceptual arrow-pushing scheme for PV electron transfer with an intervening -oxo. (b) Vanadium-P-phosphinite archetype: conceptual arrow-pushing scheme for PV electron transfer in which they are directlybound to each other.
involves both proton and electron transfer. The ROA mechanistic motif, by keeping the sites of
basicity and reduction on separate moieties, is able to decouple this process and hence allow the
best of both worlds with high basicity and high electron affinity .
The validity of the ROA mechanistic motif was tested using quantum mechanical calculations
on small X4O10 clusters, where each X is a P or V. The results, shown in Figure 4.5, indicate that
a single linkage to V makes the PO bond 32.3 kcal/mol more active, while coupling to a second V
makes it an additional 23.8 kcal/mol more active and coupling to a third V (as in VPO) makes it
an additional 4.9 kcal/mol more active. Compared to a pure vanadium (V) oxide case, coupling to
one or two P atoms makes it 13.4 and 8.5 kcal/mol more active, respectively.
Figure 4.5. Use of finite cluster models to investigate how the OH bond strength of PO moieties variesbased on the number of V coupled to it via O linkages. Data is summarized from Figure 4.8. All numbersare in kcal/mol.
a. P4O10 28.2
b. P3VO10 60.5
c. P2V2O10 84.3
d. PV3O10 89.2
e. V4O10 75.8
The data presented in Figure 4.5 shows the validity of the small cluster approach in gauging
the activity of the ROA mechanism. In hopes of expanding the chemical space in which this ROA
mechanism is available, we have undertaken an investigation of mixed oxos with vanadium and the
heavier group 15 (pnictogen) and 16 (chalcogen) elements in the first part of this chapter. (We do not
consider group 14 or 17 elements due to the instability of terminal oxos for such elements, against
hydration in the group 14 case and explosion in the group 17 case.) For each of these complexes, we
have calculated DH, the oxo-hydrogen bond energy. We use DH as a proxy for hydrogen-abstraction
potential, which is typically the most difficult step in alkane oxidation/functionalization catalysis.
We have found that the ROA mechanism is general to group 15 and 16 (pnictogen and chalcogen)
vanadium mixed oxos, with phosphorus, selenium, and tellurium being the most active. We have
also taken these most active cases, with molybdenum (VI) substituted for vanadium (V), and found
similarly promising results. We hence conclude that the reduction-coupled oxo activation mechanistic
motif is a viable and interesting new lead for the development of new oxidation catalysts.
4.2.3 Potential homogeneous catalysts utilizing the ROA principle
Although the ROA phenomenon was originally disco